Chapter 1: Dye-sensitized Solar Cells (DSCs)
1.4 Nanostructured photoanode
1.4.1 Research trends in DSC photoanodes
Nowadays, the research to improve photoanode performance is still active and is based on three main approaches :
TiO2 chemical modification;
alternative photoanode materials;
morphological optimization of the semiconductor layer.
TiO2 chemical modification
One of the major limitation of TiO2-based photanodes is the relatively slow electron diffusion through the nanocrystalline layer. It was in fact demonstrated that electron transport is slowed down by subsequent trapping and de-trapping between different electronic states. In order to overcome this limitation, and improve TiO2 performance, different approaches have been considered [12,46]. In particular, the production of composite systems, core-shell structure or element doping have been studied. Eguchi et al.  studied the TiO2-Nb2O5 composite with different compositions. The FF resulted to increase with the Nb2O5 content due to reduced recombination phenomena. Also Voc increased, thanks to the second oxide higher band gap energy (Eg). Jsc was instead
reduced for the lower surface area of Nb2O5. The TiO2-ZrO2 composite was studied by Kitiyann et al. obtaining a relevant increase in efficiency despite the decay in FF .
The configuration reported confines the electron in the TiO2 core of the system, thus reducing the recombination reactions. Palomares et al.  tested different materials as shells for DSC obtaining the best performance with Al2O3. Over a certain shell thickness however, the performance dropped due to an excessive surface area reduction limiting dye adsorption. The opposite behavior was observed with MgO, which favored an increase in the surface area an then in Jsc . The results obtained with several TiO2 modifications are summarized in Table I.
Table I. DSC performance with modified TiO2, data referring to pure TiO2 are reported in brackets.
Approach Composition VOC (mV) FF JSC
(mA/cm2) η (%)
Core / Shell
TiO2- ZrO2 675 (735) 0.60 (0.75) 9.1 (9.1) 3.6 (3.7) TiO2/Nb2O5 732 (659) 0.56 (0.51) 11.4 (10.2) 4.7 (3.5) TiO2/SiO2 710 (735) 0.58 (0.55) 10.6 (9.1) 4.4 (3.7) TiO2/Al2O3 760 (735) 0.61 (0.55) 12.1 (9.1) 5.6 (3.7) TiO2/MgO 720 (640) 0.54 (0.47) 11.7 (10.2) 4.5 (3.1) TiO2/ZnO 620 (490) 0.52 (0.40) 11.7 (13.2) 4.5 (3.3)
95TiO2-05ZrO2 670 (710) 0.72 (0.68) 11.2 (10.1) 5.8 (4.6) 80TiO
2-20Nb2O5 645 (600) 0.42 (0.29) 6.83 (7.89) 1.9 (1.4) Doping TiO2:0.1% Nb 841 (777) 0.69 (0.54) 3.1 (2.2) 1.8 (1.0) 99TiO2-1Zr 715 (700) 0.69 (0.64) 16.5 (15.6) 8.1 (7.0)
The last approach listed in Table I involves the doping of TiO2 lattice. In this context Durr and co-workers  substituted Ti4+ with Zr4+ ions, observing that ZrO2
segregation did not occur up to a 2 mol.% concentration of Zr. Doped-TiO2 cells showed a 15% increase in efficiency compared to the reference TiO2 sample. The same
trend was obtained using Nb2O5 . At last, common to all the reported studies is the doped layers dye uptake increase, with a consequent Jsc enhancement. This is mainly related to the doping process, carried out by powder chemical synthesis, during which the dopant ions in TiO2 lattice generally promote a contraction of the final particle size compared to pure TiO2, thus increasing the surface area.
Alternative photoanode materials
As extensively treated in section 1.3, the operating mechanism of DSCs is based on the spontaneous dissociation of the photogenerated exciton. This process could be only possible if the dye LUMO is located at higher energy than the CB of photoanode material. Otherwise, the electron transfer does not occur and there is no current generation. In addition, charge separation is entropycally favoured by the higher density of state in the CB of a crystal (as the photoanode material) rather than in an organic dye molecular orbital. Therefore, the correct CB position is a fundamental requisite for a material to be a candidate photoanode. The band gap energy (Eg) is another determining factor. A large value of Eg, in fact, means a high energy difference with the electrolyte potential, with a positive impact on the Voc. In addition, a large Voc helps in preventing recombination phenomena . The selection of an alternative photoanode material therefore requires a deep comprehension of its electronic properties. Figure 1.13 reports the schematization of the most common photoanode materials energy levels.
Figure 1.13. Most common anode materials bang gap energy and CB level.
Several materials have been tested as possible photoanodes. ZnO was one of the first compounds employed in sensitization studies with organic dyes [54,55]. Its electronic structure is quite similar to TiO2, with Eg of 3.37 and a Fermi level located at -4.45 V.
The most important ZnO limitation is its low compatibility with the common Ru-based dyes, due to their acidic nature that causes a rapid desorption and a relevant performance reduction. Moreover, dye molecules form aggregates on ZnO surface, compromising charge separation and collection . Finally, the relatively low value of ZnO dielectric constant (8 vs 30-170 of TiO2) may limit the exciton separation efficiency, causing a reduction in the performance. In conclusion, ZnO was also considered for the simplicity of producing several different morphologies, however it did not reach the stability and the performance of TiO2 layers .
Nb2O5 has a wider band gap than TiO2; for this reason it increases the cell Voc.
However, the overall performance is affected by the oxide crystal structure, that limits the dye loaded amount and then the efficiency .
The same positive effect on Voc is expected considering SnO2, due to its high band gap.
However this material suffers from different drawbacks when used in DSCs [58,59].
First, more rapid recombination phenomena occur due to the electron diffusion coefficient up to 100 time higher than the TiO2 one. In addition the negative shift of the conduction band may reduce and limit the electron generation and transfer. Finally, the low isoelectric point of the material (4-5) inhibits the adsorption of dyes with acidic character. A possible solution to overcome this limitation is the application of passive layer upon the SnO2 one. Using MgO for example, the performance of a SnO2-based cell registered a 7.02% efficiency .
Finally, also ternary oxides have been tested as possible TiO2 substitutes. The first was SrTiO3, having properties (as Eg and band position) similar to the ones of TiO2 .
However, the efficiency was found to be still low due to the oxide structure: the basic (001) plane is in fact exposed and its nature causes problems with acidic dyes, as reported for ZnO. Lastly, Zn2SnO4 showed interesting characteristics, such as a maximum efficiency of 3.8% (comparable to ZnO based cells) and a good stability in acidic conditions . However its main limitation is linked to the low efficiency of electron transfer and transport.
Morphological and topographical layer optimization.
Mesoporous films made of randomly oriented nanoparticles represent the paradigm of photoanodes for DSCs. When designing and producing this kind of photoelectrodes, the primary challenge is to obtain a well-dispersed, thick and crack free layer, in order to maximize its contribution to the overall cell performance. From the early development of DSCs up to now this film structure has been mainly produced by screen-printing constantly giving the best results. However, a variety of microstructures have been tested so far, basically motivated by the assumption that this common 3D structure provides a complicated pathway for electron transport, thus increasing the probability of charge recombination. In this context one dimensional (1D) morphologies are considered possible alternatives, theoretically providing direct pathways for charge transport. Hence, the research has been devoted to 1D architectures as nanotubes, nanowires, nanorods, etc. [62-70]. However, despite partially solving the afore-mentioned issues, these systems suffered from common limitations as the reduced surface area, affecting the dye loading and Jsc. Another problem is the opacity of some of these layers, that therefore requires back-side illumination. On the other hand, different 3D nanoparticles structures exhibited good potentialities, even improving the charge transport efficiency. Among them, the most relevant results were obtained using a film composed of octahedron-like TiO2 single crystals. This system recorded an efficiency of 10.2% compared to the 9.6% obtained by the common nanoparticle based electrode. Promising results were also obtained using mesoporous anatase single crystals. The most important aspect was the low temperature production (150°C) .
Finally, a network made of TiO2 nanorods showed good performance (light scattering, porosity and charge transfer) when used in conjunction with a solid hole transport material (HTM) . Working on TiO2 morphology represents the most exploited way to improve the photoanode properties but also the optimization of its topography, if well-designed, can positively affect the DSC operation. In particular, a TiO2 structure composed by ordered and spatially separated rods (or cylinders), produced by photolithography, showed positive effects on the cell current density and FF providing clear evidence that the contact area between the semiconductor oxide-based electrode and the sensitizer plays an important role on the DSC efficiency .
Based on these final evidences, this PhD work was mainly oriented to the production of 3D engineered photoanodes, composed by a mesoporous layer film covered with 3D structures, able to increase DSC performance.
 Solar Generation 6 “EPIA – European Photovoltaic Industry Association, 2011”.
 U.S. Energy Information Administration, “Annual Energy Outlook 20017”.
 J. Wu, Z. Lan, J. Lin, M. Huang, Y. Huang, L. Fan, G. Luo, Electrolyte in Dye-Sensitized Solar Cells, Chemical Reviews, 2015, 115, 2136-2173.
 L. M. Gonçalves, V. de Zea Bermudez, H. A. Ribeiro, A. M. Mendes, Dye-Sensitized solar cells: a safe bet for the future, Energy & Environmental Science, 2008, 1, 655-667.
 T. Markvart, L. Castañer, Solar Cells: Materials, Manufacture and Operation, Elsevier Edition, 2005.
 S. Mathew, A. Yella, P. Gao, R. Humpry-Baker, B. F. E. Curchod, N. Ashari-Astani, I. Tavernelli, U. Rothlisberger, Md. K. Nazeeruddin, M. Grätzel, Dye-Sensitized solar cells with 13% efficiency achieved through the molecular engineering of porphyrin sensitizers, Nature Chemistry, 2014, 6, 242-247.
 H. M. Upadhyaya, S. Senthilarasu, M. H. Hsu, D. K. Kumar, Recent progress and the status of dye-sensitized solar cell (DSSC) technology with state-of-the-art conversion efficiency, Solar Energy Materials & Solar Cells, 2013, 119, 291-295.
 V. Sugathan, E. John, K. Sudhakar, Recent improvements in dye sensitized solar cells: A review, Renewable and Sustainable Energy Reviews, 2015, 52, 54-64.
 M. Ye, X. Wen, M. Wang, J. Iocozzia, N. Zhang, C. Li, Z. Lin, Recent advances in dye-sensitized solar cells: prom photoanode, sensitizers and electrolytes to counter-electrode, Materials Today, 2015, 18, 155-162.
 K. Kalyanasundaram, Dye-Sensitized Solar Cells, 2010 (First Edition), EPFL Press Lausanne (Switzerland).
 A. Hagfeldt, G. Boschloo, L. Sun, L. Kloo, H. Pettersson, Dye-Sensitized Solar Cells, Chemical Reviews, 2010, 110, 6595-6663.
 A. Sangiorgi, R. Bendoni, N. Sangiorgi, A. Sanson, B. Ballarin, Optimized TiO2
blocking layer for dye-sensitized solar cells, Ceramics International, 2014, 40, 10727-10735.
 H. J. Snaith, Estimating the maximum attainable efficiency in Dye-Sensitized Solar Cells, Advanced Functional Materials, 2010, 20, 13-19.
 B. E. Hardin, H. J. Snaith, M. D. McGehee, The renaissance of dye-sensitized solar cells, Nature Photonics, 2012, 6, 162-169.
 M. Grätzel, Dye-sensitized solar cells, Journal of Photochemistry and Photobiology C: Photochemistry Reviews, 2003, 4, 145-153.
 P. J. Cameron, L. M. Peter, Characterization of titanium dioxide blocking layers in dye-sensitized nanocrystalline solar cells, Journal of Physical Chemistry B., 2003, 107, 14394-14400.
 A. Jena, S. P. Mohanty, P. Kumar, J. Naduvth, V. Gondane, P. Lekha, J. Das, H. K.
Narula, S. Mallick, P. Bhargava, Dye Sensitized Solar Cells: a Review, Transactions of the Indian Ceramic Society, 2012, 71:1, 1-16.
 C. P. Cho, H. Y. Wu, C. C. Lin, Impacts of sputter-deposited platinum thickness on the performance of dye-sensitized solar cells, Electrochimica Acta, 2003, 107, 488-493.
 G. Syrrokostas, A. Siokou, G. Leftheriotis, P. Yianoulis, Degradation mechanisms of Pt counter electrodes for dye-sensitized solar cells, Solar Energy Materials and Solar Cells, 2012, 103, 119-127.
 J. G. Nam, Y. J. Park, B. S. Kim, J. S. Lee, Enhancement of efficiency of dye-sensitized solar cell by utilizing carbon nanotube counter electrode, Scripta Materialia, 2010, 62, 148-154.
 E. Ramasamy, W. J. Lee, D. Y. Lee, J. S. Song, Spray coated multi-wall carbon nanotube counter electrode for tri-iodide reduction in dye-sensitized solar cells, Electrochemistry Communications, 2008, 10, 1087-1089.
 S. Yun, A. Hagfeldt, T. Ma, Pt-free counter electrode for Dye-Sensitized Solar Cells with high efficiency, Advanced Materials, 2014, 26, 6210-6237.
 J. Theerthagiri, A. R. Senthil, J. Madhavan, T. Maiyalagan, Recent progress in non-platinum counter electrode materials for Dye-Sensitized Solar Cells, ChemElectroChem, 2015, 2, 928-945.
 S. Thomas, T. G. Deepak, G. S. Anjusree, T. A. Arun, S. V. Nair, A. S. Nair, A review on counter electrode materials in dye-sensitized solar cells, Journal of Materials Chemistry A, 2014, 2, 4474-4490.
 X. Zheng, J. Guo, Y. Shi, F. Xiong, W. H. Zhang, T. Ma, C. Li, Low-cost and high-performance CoMoS4 and NiMoS4 counter electrodes for dye-sensitized solar cells, Chemical Communications, 2013, 49, 9645-9647.
 M. Wu, X. Lin, Y. Wang, L. Wang, W. Guo, D. Qi, X. Peng, A. Hagfeldt, M.
Grätzel, T. Ma, Economical Pt-free catalysts for counter-electrodes of dye-sensitized solar cells, Journal of American Chemical Society, 2012, 134, 3419-3428.
 S. Yun, L. Wang, W. Guo, T. Ma, Non-Pt counter electrode catalysts using tantalum oxide for low-cost dye-sensitized solar cells, Electrochemistry Communications, 2012, 24, 69-73.
 C. Bu, Q. Tai, Y. Liu, S. Guo, X. Zhao, A transparent and stable polypyrrole counter electrode for dye-sensitized solar cell, Journal of Power Source, 2013, 221, 78-83.
 X. Zhang, S. Wang, S. Lu, J. Su, T. He, Influence of doping anions on structure and properties of electro-polymerized polypyrrole counter electrodes for use in dye-sensitized solar cells, Journal of Power Source, 2014, 246, 491-498.
 L. Y. Chang, C. T. Li, Y. Y. Li, C. P. Lee, M. H. Yeh, K. C. Ho, J. J. Lin, Morphological influence of polypyrrole nanoparticles on the performance of dye-sensitized solar cells, Electrochimica Acta, 2015, 155, 263-271.
 D. K. Hwang, D. Song, S. S. Jeon, T. H. Han, Y. S. Kang, S. S. Im, Ultrathin polypyrrole nanosheets doped with HCl as counter electrodes in dye-sensitized solar cells, Journal of Materials Chemistry A, 2014, 2, 859-865.
 J. Wu, Y. Li, Q. Tang, G. Yue, K. Lin, M. Huang, L. Meng, Bifacial dye-sensitized solar cells: a strategy to enhance overall efficiency based on transparent polyaniline electrode, Scientific Reports, 2014, 4, 4028.
 P. Chawla, M. Tripathi, Novel improvements in the sensitizers of dye-sensitized solar cells for enhancement in efficiency-a review, International Journal of Energy Research, 2015, 39, 1579-1596.
 M. R. Narayan, Review: Dye sensitized solar cells based on natural photosensitizers, Renewable and Sustainable Reviews, 2012, 16, 208-215.
 F. Bella, C. Gerbaldi, C. Barolo, M. Grätzel, Aqueous dye-sensitized solar cells, Chemical Society Reviews, 2015, 44, 3431-3473.
 A. F. Nogueira, C. Longo, M. A. De Paoli, Polymers in dye sensitized solar cells:
overview and perspectives, Coordination Chemistry Reviews, 2004, 248, 1455-1468.
 M. Wang, N. Chamberland, L. Breau, J-E. Moser, R. H-Baker, B. Marsan, S. M.
Zakeeruddin, M. Grätzel, An organic redox electrolyte to rival triiodide/iodide in dye-sensitized solar cells, Nature Chemistry, 2010, 2, 385-389.
 L. Li, X. Yang, J. Zhao, J. Gao, A. Hagfeldt, L. Sun, Efficient organic dye sensitized solar cells based on modified sulfide/polysulfide electrolyte, Journal of Materials Chemistry, 2011, 21, 5573-5575.
 M. Pelaez, N. T. Nolam, S. C. Pillai, M. K. Seery, P. Falaras, A. G. Kontos, P. S.
M. Dunlop, J. W. J. Hamilton, J. A. Byrne, K. O‟Shea, M. H. Entezari, D. D.
Dionysiou, A review on the visible light active titanium dioxide photocatalysts for environmental applications, Applied Catalysis B: Environmental, 2012, 125, 331-349.
 R. Jose, V. Thavasi, S. Ramakrishma, Metal oxide for dye-sensitized solar cells, Journal of the American Ceramic Society, 2009, 92, 289-301.
 B. O‟Regan, M. Grätzel, A low cost, high efficiency solar cell based on dye sensitized colloidal TiO2 films, Nature, 1991, 353, 737-740.
 M. Grätzel, Solar energy conversion by dye-sensitized photovoltaic cells, Inorganic Chemistry, 2005, 44, 6841-6851.
 Y. Bai, I. Mora-Sero, F. De Angelis, J. Bisquert, P. Wang, Titanium dioxide nanomaterials for photovoltaic applications, Chemical Reviews, 2014, 114, 10095-10130.
 R. Beranek, (Photo)electrochemical methods for the determination of the band edge positions of TiO2-based nanomaterials, Advances in Physical Chemistry, 2011.
 K. Eguchi, H. Koga, K. Sekizawa, K. Sasaki, Nb2O5-based composite electrodes for dye-sensitized solar cells, Journal of the Ceramic Society of Japan, 2000, 108, 1067-1071.
 A. Kitiyanan, S. Yoshikawa, The use of ZrO2 mixed TiO2 nanostructures as efficient dye-sensitized solar cell’s electrodes, Materials Letter, 2005, 59, 4038-4040.
 E. Palomares, J. N. Clifford, S. A. Haque, T. Lutz, J. R. Durrant, Control of charge recombination dynamics in dye sensitized solar cells by the use of conformally deposited metal oxide blocking layers, Journal of the American Ceramic Society, 2003, 125, 475-482.
 A. Zaban, S. G. Chen, S. Chappel, B. A. Gregg, Bilayer nanoporous electrodes for dye sensitized solar cells, Chemical Communications (Cambridge), 2000, 22, 2231-2232.
 M. Durr, S. Rosselli, A. Yasuda, G. Nelles, Band-gap engineering of metal oxides for dye-sensitized solar cells, The Journal of Physical Chemistry B, 2006, 110B, 21899-21902.
 H. Jung, J. K. Lee, M. Nastasi, S. W. Lee, J. Y. Kim, J. S. Park, K. S. Hong, H.
Shin, Preparation of nanoporous MgO-coated TiO2 nanoparticles and their application to the electrode of dye-sensitized solar cells, Langmuir, 2005, 21, 10332-10335.
 S. Roh, R. S. Mane, S. Min, W. Lee, C. D. Lokhande, S. Han, Achievement of 4.51% conversion efficiency using ZnO recombination barrier layer in TiO2 based dye-sensitized solar cells, Applied Physics Letters, 2006, 89, 253512.
 G. Redmond, D. Fitzmaurice, M. Grätzel, Visible light sensitization by Cis-Bis (thiocyanato) Bis (2,2’-bipyridyl-4.4’-dicarboxylato) Ruthenium(II) of transparent nanocrystalline ZnO films prepared by sol-gel techniques, Chemistry of Materials, 1994, 6, 686-691.
 H. Rensmo, K. Keis, H. Lindstrom, S. Sodergren, A. Solbrand, A. Hagfeldt, S. E.
Lindquist, L. N. Wang, M. Muhammed, High light-to-energy conversion efficiencies for solar cells based on nanostructured ZnO electrodes, The Journal of Physical Chemistry B, 1997, 101, 2598-2601.
 K. Keis, J. Lindgren, S. E. Lindquist, A. Hagfeldt, Studies of the adsorption process of Ru complexes in nanoporous ZnO electrodes, Langmuir, 2000, 16, 4688-4694.
 P. Guo, M. A. Aegerter, Ru(II) sensitized Nb2O5 solar cell made by the sol gel process, Thin Solid Films, 1999, 351, 290-294.
 E. Ramasamy, J. Lee, Ordered mesoporous SnO2-based photoanodes for high performance dye-sensitized solar cells, The Journal of Physical Chemistry C, 2010, 114, 22032-22037.
 M. K. I. Senevirathna, P. K. D. D. P. Pitigala, E. V. A. Premalal, K. Tennakone, G.
R. A. Kumara, A. Konno, Stability of the SnO2/MgO dye-sensitized photoelectrochemical solar cell, Solar Energy Materials and Solar Cells, 2007, 91, 544-547.
 P. Balaya, J. Jamnik, J. Fleig, J. Maier, Mesoscopic electrical conduction in nanocrystalline SrTiO3, Applied Physics Letters, 2006, 88.
 B. Tan, E. Toman, Y. Li, Y. Wu, Zinc stannate (Zn2SnO4) dye sensitized solar cells, Journal of the American Ceramic Society, 2007, 129, 4162-4163.
 J. M. Macak, H. Tsuchiya, A. Ghicov, P. Schmuki, Dye-sensitized anodic TiO2
nanotubes, Electrochemistry communications, 2005, 7, 1133-1137.
 J. H. Park, T. W. Lee, M. G. Kang, Growth, detachment and transfer of highly-ordered TiO2 nanotube arrays: use in dye-sensitized solar cells, Chemical Communications, 2008, 25, 2867-2869.
 K. Zhu, N. R. Neale, A. Miedaner, A. J. Frank, Enhanced charge-collection efficiencies and light scattering in dye-sensitized solar cells using oriented TiO2
nanotube arrays, Nano Letters, 2007, 7, 69-74.
 J. Jiu, S. Isoda, F. Wang, M. Adachi, Dye-sensitized solar cells based on a single-crystalline TiO2 nanorod film, The Journal of Physical Chemistry B, 2006, 110, 2087-2092.
 B. Liu, E. S. Aydil, Growth of oriented single-crystalline rutile TiO2 nanorods on transparent conducting substrates for dye-sensitized solar cells, Journal of the American Chemical Society, 2009, 131, 3985-3990.
 H. Wang, M. Liu, M. Zhang, P. Wang, H. Miura, Y. Cheng, J. Bell, Kinetics of electron recombination of dye-sensitized solar cells based on TiO2 nanorods arrays sensitized with different dyes, Physical Chemistry Chemical Physics, 2011, 13, 28, 17359-17366.
 E. Enache-Pommer, J. E. Boercker, E. S. Aydil, Electron transport and recombination in polycrystalline TiO2 nanowire dye-sensitized solar cells, Applied Physics Letters, 2007, 91, 123116.
 X. Feng, K. Zhu, A. J. Frank, C. A. Grimes, T. E. Mallouk, Rapid charge transport in dye-sensitized solar cells made from vertically aligned single-crystal rutile TiO2
nanowires, Angewandte Chemie International Edition, 2012, 51, 2727-2730.
 J. Y. Liao, B. X. Lei, H. Y. Chen, D. B. Kuang, C. Y. Su, Oriented hierarchical single crystalline anatase TiO2 nanowire arrays on Ti-foil substrate for efficient flexible dye-sensitized solar cells, Energy and Environmental Science, 2012, 5, 5750-5757.
 J. W. Shiu, C. M. Lan, Y. C. Chang, H. P. Wu, W. K. Huang, E. W. Diau, Size-controlled anatase titania single crystals with octahedron-like morphology for dye-sensitized solar cells, ACS Nano, 2012, 6, 10862-10873.
 E. J. W. Crossland, N. Noel, V. Sivaram, T. Leijtens, J. Alexander-Webber, H. J.
Snaith, Mesoporous TiO2 single crystals delivering enhanced mobility and optoelectronic device performance, Nature, 2013, 495, 215-219.
 T. H. Meen, C. J. Huang, Y. W. Chen, L. W. Ji, C. C. Diao, H. H. Chung, Study of different TiO2 electrode structures on Dye-Sensitized Solar Cell, Key Engineering Materials, 2008, 368-372, 1716-1719.